Application Technique : BL Exhaust Coat
There is no need to dilute it.
Apply the primer color, final coat heat resistant clear, and paint undiluted.
1Completely remove all debris and foreign substances from the item’ s surface
Completely degrease the item to be painted, and carry out the surface preparation and base polishing.
2Paint the primer color
We recommend that you apply the primer color as thin as possible.
Maintain the previously set temperature of the baking pot at 70°C~80°C.
After you paint the primer color, maintain the temperature of the item at 180°C~190°C while baking it for 30 minutes.
After this, cool down the item until it returns to a normal temperature.
3Paint the heat resistant clear
Once again, maintain the set temperature of the baking pot at 70°C~ 80°C.
Maintain the temperature of the item at 180°C~ 190°C while baking it for 30 minutes.
The BL Exhaust Coat (Heat Resistant 2 Coat System) provides an extremely thin coat, so if it gets mixed with debris or foreign substances, cracking or peeling make occur after it finishes baking. Because of this, make sure to completely remove all debris and carefully prepare the surface.
Carry out this work in an environment that has less than 70% humidity.
Standard thickness of the BL Exhaust Coat system
Undercoat color thickness: 20 ~ 30μm (micrometers) = 0.02 to 0.03 mm Overcoat clear thickness: 5 ~ 10μm (micrometers) = .005 to 0.01 mm
Overcoat heat clear coat : Data obtained from a performance test on film
100 hours heating/discoloration, no peeling or cracking during the heat resistance test at 300°C. Gloss retention rate of 95% or more.
Hardness : 8 ~ 9H
Oil resistance test
After 3 hours in contact with gasoline in a single spot 20oC the coating film did not present any abnormality after checking it visually.
After 48 hours immersion in kerosene at 20oC the coating film did not present any abnormality after checking it visually.
After 3 hours in contact with engine oil in a single spot at 20oC the coating film did not present any abnormality after checking it visually.
Water resistance test
After 24 hours immersion in boiling water, the coating did not present any abnormality.
Stain resistance test
After writing with permanent maker pen(black, red, blue)and wiping it with a dry cloth, there were no abnormalities.
Performed with a gas burner open flame for 20 seconds. Test result: Incombustible.
* Conducted under the following conditions //
Material : SUS304 / Film thickness3~5μm / Curing conditions 180°C × 30min.
* The above figures are reference values, not a standard value.
1 mm grid test : This is a test to check adhesion performance of BL Exhaust Coat
This is a test to check the heat resistance performance of BL Exhaust Coat.
Excellent deformation following performance test of BL Exhaust Coat.
How to Order
Paint in general is treated as hazardous goods, so for shipping charges, we must make individual estimates by airline according to country and region.
We will then send you a bill including those shipping charges via paypal. After checking that amount, please decide whether or not to purchase our products.
paypal is our only payment method. You can cancel the order at any time.
Furthermore, please note that it will be about 10~14 days before items are shipped.
Estimated shipping charges
Forwarder & Transportation : ANA cargo or K-Line Logistics
The minimum fee is set for international transportation of dangerous goods.
The following is the minimum fee in each region.
Central America : 55,000〜65,000JPY
South America : 75,000〜85,000JPY
Europe / Russia : 60,000〜75,000JPY
India / Middle east : 75,000〜85,000JPY
Africa : 65,000〜85,000JPY
Recruiting Distributors & Dealers
PRESENCE Co., Ltd. / BADLAND
4-18-1 Minamikase Saiwaiku Kawasaki Kanagawa JAPAN
ZIP CODE : 212-0055
TEL +81-44-587-3139 / FAX +81-44-580-3431 / e-mail : firstname.lastname@example.org